FACOLTÀ DI SCIENZE MATEMATICHE FISICHE E NATURALI
Dottorato in Scienze Chimiche
XXIII ciclo (2008 - 2010)
CHARGE AND ENERGY TRANSFER IN FUNCTIONAL MOLECULAR MATERIALS:
SPECTROSCOPY AND MODELS
Prof. Alberto Girlando
Prof. Anna Painelli Prof. Alberto Girlando
Dottorando Luca Grisanti
List of Abbreviations V
1 CT chromophores and multichromophores: essential state models
and spectroscopic behaviour 5
1.1 Essential state description of a DA chromophore . . . 6
1.2 Essential state models for chromophore and multichromophore . 13 DAchromophores beyond the two state approach . . . 14
1.3 Terpyridine-based ligand and the related Zn-complex . . . 15
1.3.1 Ligand: spectroscopy and two state model . . . 15
1.3.2 Optical spectra of [ZnT]: the need for an extension of the model . . . 16
1.4 Annine: CT vs localized excitations . . . 25
1.4.1 Optical properties of An . . . 25
1.4.2 Optical properties of NAn . . . 26
1.4.3 CT and localized transition and the failure of the standard two-state approach . . . 31
1.4.4 A three state model for the two transitions in NAn . . . 32
1.4.5 Results . . . 35
1.4.6 Experimental properties of NAnMe+ . . . 40
Interacting polar chromophores . . . 43
1.5 Dimers of polar chromophores in solution: stilbazole and bipyridine 43 1.5.1 Stilbazole: the two state model at work . . . 44
1.5.2 Interacting dipolar chromophore: bipyridine . . . 47
1.5.3 Optical spectra for bipyridine along bottom-up modelling . 51 1.5.4 Ab initio and TDDFT calculated absorption and TPA prop- erties . . . 55
1.5.5 Bottom up essential state modelling and ab initio results in calculating spectral properties and to understand the
role of the interaction . . . 58
1.6 Dipolar DA fluorenes and related spirobifluorenes: bichromophores beyond the electrostatic interactions . . . 60
1.6.1 Experimental optical properties . . . 61
1.6.2 Modeling fluorenes and spirobifluorenes: a bottom-up ap- proach . . . 66
1.6.3 Results . . . 73
1.6.4 Fluorescence anisotropies, excitation and emission spec- tra in frozen solvent . . . 80
1.6.5 Understanding the red edge effect . . . 90
1.7 Conclusion . . . 92
2 Mixed valence systems and bistability 93 2.1 FcPTM and FcMe9PTM: from solution spectra to bistability in molecular crystals . . . 94
2.1.1 Solution spectra and two state model . . . 95
2.1.2 Bistability in FcPTM crystal: the electronic model . . . 100
2.1.3 Bistability in FcPTM crystals: the complete model . . . 104
2.1.4 Bistability in FcPTM crystals: estimating the Madelung energy . . . 106
2.1.5 Bistability in FcPTM crystal: Mössbauer spectra . . . 109
2.1.6 FcMe9PTM in solution: the need for a three state model . 112 2.1.7 The role of low energy bridge states . . . 117
2.1.8 Three-state models for bistability . . . 121
2.2 FcPyl+-based materials: extending the bistability model to ionic crystals . . . 124
2.2.1 The model for a molecular ion crystal . . . 125
2.2.2 Results . . . 127
2.3 TTFPTM• and related systems: bistability and aggregation phe- nomena . . . 134
2.3.1 TTFPTM: bistability in solution . . . 134
2.3.2 Dimers of TTFPTM and derivatives . . . 139
2.4 Conclusion . . . 149
3 Electron-phonon coupling in molecular organic semiconductors 151 3.1 The calculation of carrier-phonon coupling constants in organic semiconductors . . . 152
3.1.1 Phonon structure . . . 153
3.1.2 Electronic structure . . . 154
3.1.3 Carrier-phonon coupling . . . 156
3.2 The rubrene crystal . . . 158
3.2.1 The crystal structure of rubrene . . . 158
3.2.2 Rubrene transfer integrals and coupling constants . . . 159
3.2.3 Discussion . . . 172
3.3 Conclusions and further developments . . . 174
4 Resonant energy transfer and chromophore excitation interactions 177 4.1 Common theoretical treatment for resonance energy transfer . . . 179
4.1.1 The transition densities approach . . . 179
4.1.2 The dipolar approximation and experimentally accessible information . . . 179
4.2 Semiempirical MO-CIS approaches to energy transfer . . . 182
4.2.1 Frozen orbitals MO-CIS evaluation of V with INDO/S Hamil- tonian . . . 182
4.2.2 From transition densities to point atomic charge densities in the INDO/S . . . 185
4.3 Extended dipole methods in essential state models . . . 186
4.4 Results . . . 186
4.5 Conclusion and further developments . . . 193
A Experimental techniques 199 A.1 Absorption and Fluorescence . . . 199
A.1.1 Measurement of fluorescence quantum yields (FQY) . . . . 199
A.1.2 T dependent optical Vis-NIR-MIR measurements . . . 201
A.2 Two photon absorption (TPA) and two-photon excited fluores- cence (TPEF) . . . 201
A.3 Cryogenic measurements on solutions . . . 202
A.3.1 Cryostat and experimental setup . . . 203
A.3.2 Glassy solution measurements . . . 205
A.4 Fluorescence anisotropy . . . 206
A.4.1 Fundamental aspects and experimental setup for anisotropy measurements . . . 206
B Computational details for the calculation of optical spectra 211 B.1 Calculation of absorption and fluorescence spectra . . . 211
B.1.1 Spectra calculation in the non-adiabatic approach . . . 211
B.1.2 Spectra calculation in the adiabatic approximation . . . 212
B.2 Calculation of the two-photon absorption spectra . . . 214
B.3 Calculation of emission and excitation anisotropy . . . 215
B.3.1 Calculation of anisotropy spectra . . . 215
B.3.2 Anisotropy calculation with orientational degree of freedom217 C The MO-CIS approach for excited state description and the INDO/S semiempirical method 219 C.1 HF-MO frame . . . 219
C.2 CIS: the simplest approach for excited states . . . 220
C.3 Semiempirical method: INDO/S . . . 221
C.3.1 Zerner INDO/S approximations and expressions . . . 221
C.3.2 INDO/S and CIS method . . . 223
C.3.3 INDO/S transition and permanent dipole moment . . . 224
List of Publications 239
List of Abbreviations
CT charge transfer
D/ A electron donor/acceptor (group)
D/A energy donor/acceptor (molecule)
LE localized excitation
NLO nonlinear optics
mv/e-mv molecular vibration/electron-mv
PES potential energy surface
OPA one-photon absorption
TPA two-photon absorption
TPEF two-photon excited fluorescence
GM Göppert-Mayer units(1GM=10−50· cm4· s · photon−1)
mf mean field
gs, g ground state
a. u. arbitrary units
ET energy transfer
RET resonant energy transfer
(N)IR (near) infrared
XRD X ray diffraction
MO molecular orbital
HF Hartree Fock
INDO intermediate neglect of differential overlap INDO/S, ZINDO INDO with spectroscopic parametrization
CI configuration interaction
CIS single excited configuration interaction HOMO highest occupied molecular orbital LUMO lowest unoccupied molecular orbital
PCM polarizable continuum model
(TD)DFT (time dependent) density functional theory
RMA rigid molecule approximation
QHLD quasi harmonic lattice dynamics
The progress in chemical synthesis and the development of new organic and inorganic molecular systems is playing an important role in scientific and tech- nological innovation. Molecular-based materials are in demand for the devel- opment of new electronic and photonic devices [1, 2, 3] but also for a wealth of other applications including, to cite a few, drug delivery , in vivo optical microscopy , microfabrication [5, 6, 7], photodynamic therapy [8, 9, 10].
In particular, fundamental biological processes involve functional molecules, as best demonstrated by light harvesting complexes exploited in the photosyn- thetic process [11, 12]. A thorough understanding of these processes will unveil some fundamental mechanism of life, offering at the same time important clues for the optimal engineering of molecular- based devices . The low cost and the large availability of the organic precursors, and the possibility to build structures with unlimited complexity and finely tuned properties make molec- ular functional materials extremely appealing from a fundamental and applica- tive point of view. Functional behaviour is accompanied in molecular materials by low weight and mechanical flexibility opening the way to applications that are precluded to more common inorganic and crystalline materials used in the electronic industry. Bio-compatibility makes molecular materials useful in life- science, biological and medical applications [8, 4].
Functional molecular materials are by definition smart materials: they are able to respond in a qualitative different way to wide range of external pertur- bation: temperature, light, pressure, magnetic and electric field, etc. [3, 14, 15, 16, 17]. Smart behaviour is related to the intrinsic non-linearity of the material responses to applied perturbations that, in its extreme manifestation, lead to switchable materials.
To fully exploit the promise of molecular functional materials, the physics that governs their complex behaviour must be thoroughly understood, with the aim, on one side, to optimize the materials for current needs, on the other side to guide the synthesis of new materials showing brand new behaviour. This
thesis offers a contribution to the rationalization of the properties of several families of molecular functional materials. Systems of interest range from or- ganic and organometallic chromophores and multichromophores, valence tau- tomeric systems, bistable molecular materials, organic semiconducting crystals.
Phenomena of interest range from linear and non-linear optical spectra, charge transfer and charge transport processes, energy transfer, multistability. Differ- ent systems with distinctively different properties have been investigated adopt- ing a variety of techniques, including spectroscopic measurements, theoretical models and computational approaches.
Spectroscopic techniques include standard absorption and fluorescence spec- troscopic measurements mainly in solution. Special skills were developed in low-temperature and in frozen solution spectroscopic measurements, including fluorescence anisotropy. From the theoretical perspective large emphasis was put in the development of essential state model to describe low-energy linear and non-linear spectra of CT chromophores and multichromophores. Essential state models adopt a minimal basis to describe electronic degrees of freedom of CT chromophores just accounting for the charge-resonance that dominate the low-energy physics of these systems. Thanks to this minimal choice for the elec- tronic structure, essential state models can describe fairly accurately the cou- pling of electrons with molecular vibrations and can be extended to account for the interaction with the solvent. In a bottom-up modeling strategy, essentials state models developed for chromophores in solution offer the basis to con- struct more complex models for systems where several chromophores interact via electrostatic forces, including multichromophoric assemblies and molecular crystals.
Essential state models are semiempirical and a careful analysis of experimen- tal data is the basis for their definition. Their actual exploitation requires the development of ad hoc numerical codes, that can deal with electron-vibration coupling either adopting the adiabatic approximation or in truly non-adiabatic approaches. The codes are simple for simple systems, but become more and more complex and demanding as long as the number of slow degrees of free- dom (either molecular vibrations or polar solvation coordinates) increases. Es- sentials states models were also the basis to build models for bistable molecu- lar crystals, where the cooperative nature of the interactions was captured via a mean-field treatment of electrostatic intermolecular interactions. Quantum chemical calculations were exploited is several cases to support essential state models, and an original implementation of an INDO code was developed to at- tack in a new perspective two important and timely issues: charge transport in
organic molecular crystals and energy transfer between organic chromophores.
This extensive and multifaceted work was often done in collaboration with other groups. Notable in this respect are the collaborations with two Italian groups expert in the synthesis of organic and organometallic chromophores and multichromophores, Prof. D. Roberto (“Università degli Studi di Milano”) e Dr.
S. Quici (CNR - Milano); with an Italian group expert in non-linear optical spec- troscopy (Prof. C. Ferrante, “Università di Padova”). Another national collabo- ration was active with the group of Bologna University. The group has a well recognised expertise in optical spectroscopy of organic crystals (Prof. Brillante) and in theoretical model for the structural and vibrational properties of organic crystals (Prof. Della Valle and Venuti). Joining these expertise with the exper- tise of the host research group in modelling electronic and electron-vibration coupling in molecular materials was instrumental to attack the complex prob- lem of the in charge transport in organic semiconductors. Particularly important have been two international collaborations. The first with the group of Prof. J.
Veciana (Barcellona), that has a well recognized expertise in the synthesis and characterisation of molecular functional materials, has been supported by “EU- NOE MAGMANET”. I spent 6 weeks in Barcelona and PhD student from there spent two months in our laboratory. The second international collaboration was with the group of Prof. S. Pati (Bangalore) that is a recognized expert in the theoretical description of molecular functional materials. In the framework of this collaboration, supported by the Executive Program of Scientific and Tech- nological cooperation between the Italian Republic and the Republic of India 2008-2010, I spent a month in the laboratory of Prof. Pati.
The thesis is organized as follow. The first chapter is mainly devoted to CT chromophores and multichromophores. Essential state models are presented and exploited to describe optical spectra of several donor-acceptor (DA) chro- mophores and bichromophoric assemblies in solution. Essential state models for DAchromophores were already developed in the host laboratory [18, 19] and successfully applied to many systems [20, 21, 22, 23]. Here special emphasis is put on specific DA chromophores which spectral behaviour calls for some exten- sion of the basic model to account for the presence of several low-energy exci- tations and/or for additional slow degrees of freedom. Interchromophore inter- actions are at the hearth of models for bichromophoric systems, and have been extensively investigated in the framework of the bottom-up modelling strategy.
Extended models demand for extended spectroscopic characterization and the technique of fluorescence anisotropy, recently implemented in the host labora- tory, proved extremely successful in this context.
Chapter two describe a class of organic and metallorganic DA compounds that, with respect to the typical DA chromophores described in Chapter 1, are characterized by a low degree of conjugation between the D and A groups and therefore by weak CT absorption band occurring in the near-infrared spectral region. This family of chromophores is particularly promising for bistability . A bottom-up modeling strategy is adopted to model bistable molecular crystals of DA chromophores. The work starts with a detailed analysis of op- tical spectra of the DA dye in solution to extract the relevant molecular model that is then used to build models for interacting chromophores in the crystal.
The calculation of electrostatic intermolecular interactions is based on an orig- inal implementation of quantum chemical calculations, where a constant elec- tric field is imposed to force the molecule in one of the resonating structure and hence evaluate the relevant charge distribution. A mean-field treatment of electrostatic intermolecular interactions then proves that bistability can be induced in crystals of DA chromophores via a careful balance of inter and intra- molecular energies. The model is validated via a quantitative comparison with temperature-dependent Mössbauer spectra for a specific system. The model, originally developed from crystal of neutral DA chromophores is then extended to treat crystal of DA+ molecular ions. This non-trivial extension suggests that the electrostatic interaction between the DA+ ion and the counterion offers a powerful tool to drive the system in the bistability region. While mainly de- voted to bistability, chapter 2 touches upon other problems as well. Among them we point at the discussion of the role of bridge in D π A chromophores. Fi- nally preliminary results are discussed about a new family of DA chromophores showing an intriguing and complex physics that includes bistability in solution, dimerization equilibria and the formation of mixed-valence dimers.
In chapter three we describe a computational tool to evaluate the electron - phonon couplings in organic molecular material. The method, which involves a semiempirical quantomechanic approach, fully accounts for the mixing be- tween intramolecular and intermolecular (lattice) vibrations. The method is applied to the case of rubrene, which presents many low frequency vibrations that potentially couples with low frequency lattice phonons.
In chapter four, a short review of the resonance energy transfer mechanism is given and an original computational method based on INDO/S calculation of configuration interaction matrix elements is proposed. The computational scheme is then tested on a few pairs of organic chromophores.
CT chromophores and multichromophores:
essential state models and spectroscopic behaviour
In this chapter we focus attention on optical spectra of charge transfer (CT) chromophores and multichromophores. CT chromophores are an interesting class of π -conjugated molecules decorated with electron donor (D) and ac- ceptor (A) groups. In these molecules π conjugated electrons guarantee for low-lying excitations and large transition dipole moments, and therefore large (hyper)polarizabilities. These interesting properties are further amplified by the presence of D and A groups that lower the energy of CT states. Indeed the low energy physics of CT chromophores is governed by CT degrees of freedom, a feature exploited in the host laboratory to develop essential state models for optical spectra of CT chromophores .
CT chromophores represent a vast family of molecules: the simplest struc- ture has a D and an A group joint by a π-conjugated bridge. These polar struc- tures, also known as push-pull chromophores, have been quite extensively in- vestigated for their large NLO properties [26, 17]. Their low-frequency ab- sorption transition has a CT character and its large solvatochromism is well known . More complex and highly symmetrical chromophores include quadrupolar, D π Aπ D or Aπ D π A, and octupolar (DA3 or AD3) chromophores [28, 29, 30]. In all cases the low energy physics of these dyes is governed by CT
6 Essential state models
processes and their optical spectra can be accurately described in terms of essen- tial state models . Specifically, polar dyes resonate between two structures, DA ←→ D+A−, and the essential state model just accounts for two electronic basis states . Quadrupolar dyes can instead be described based on three electronic states , while four basis states are essential to describe octupolar dyes . The interaction with the solvent and with molecular vibrations are introduced in essential state models, leading to a fairly accurate description of solution spectra [31, 32, 33, 21, 34, 35, 36].
The same essential state models lead themselves quite naturally to describe multichromophoric assemblies [25, 37, 38, 23], where different CT chromophores interact via electrostatic forces. Essential state models have been developed in the host laboratories in the last 15 years and have been quite successfully ap- plied to many chromophores and multichromophores. However, in an effort to extend the library of molecules described in terms of essential state models, a few intriguing examples of chromophores have been encountered for which a detailed description of optical spectra requires some extension of the basic es- sential state model. In this chapter I will discuss a few examples of polar dyes where an extension of the two state model is in order, as well as a few examples of multichromophoric species.
1.1 Essential state description of a DA chromophore
The low energy physic of DA chromophore is governed by the resonance DA ←→
D+A−. The minimal model for their electronic structure then accounts for two basis state: the neutral |DA〉 state and the zwitterionic |D+A−〉 state [18, 19, 39, 33]. The Hamiltonian reads:
where 2z0 represents the energy difference between the two structures and τ is the mixing element. The same Hamiltonian is conveniently rewritten using a couple of operators:
ˆ ρ =
0 0 0 1
ˆ σ =
0 1 1 0
Hel=2z0ρ − τ ˆˆ σ (1.2)
The solution of the electronic 2 × 2 Hamiltonian is exact, and the ground and the excited state are:
|g〉 = p1 − ρ |DA〉 + pρ |D+A−〉 (1.3)
|e〉 = −pρ |DA〉 +p1 − ρ |D+A−〉 (1.4) where ρ is the expectation value in the ground state of the ˆρ operator and cor- responds to the degree of charge transferred from D to A (also called ionicity), that can vary from 0 to 1. The ρ value only depends on z0and τ:
ρ = 1 2
1 − z0 pz02+τ2
Molecules in a state characterised by ρ ≪ 0.5 (ρ ∼ 0) are in neutral regime.
Molecules with ρ ≫ 0.5 (ρ ∼ 1) are in the ionic regime. Figure 1.1 shows the ρ(z0)curves calculated for a few τ values.
-2 -1 0 1 2
z0 (a.u.) 0
0.2 0.4 0.6 0.8 1
τ = 0.0 τ = 0.1 τ = 0.5 τ = 1.0 τ = 2.0 τ = 5.0
Figure 1.1: The z0dependence of ρ for different τ values. Notice that the mixing element τ is responsible for the smoothness of the ρ(z0)curve. For τ = 0 the system can only be found at ρ = 0 or ρ = 1, and states with intermediate ionicities are only possible for finite τ.
According to the original idea of Mulliken , we neglect all matrix ele- ments of the dipole moment operator except µ0, the dipole moment in the D+A− state. The dipole moment operator then reads:
µ = µ0ρˆ (1.6)
8 Essential state models
All spectroscopically relevant quantities can be easily expressed as a function of ρ, as follows:
ρ 1 − ρ
pρ 1 − ρ (1.8)
The ρ dependence of µge and ωgeis shown in fig. 1.2. The permanent ground and excited state dipole moments are:
µg=µ0ρ µe=µ0(1 − ρ) (1.9) The solvatochromism is governed by the mesomeric dipole moment:
∆µ = µe− µg=µ0 1 − 2ρ (1.10) In particular, for a pure electronic model, the absorption solvatochromism is determined by µg∆µ and emission solvatochromism by µe∆µ.
0 0.2 0.4 0.6 0.8 1
µCT 2 (µ0 unit)
0 4 8
ωCT (τ unit)
Figure 1.2: Calculated frequency (upper panel) and square of the transition dipole moment (lower panel) of the CT transition, as a function of ρ. At ρ ∼ 0 (largely neutral molecules) or ρ ∼ 1 (largely ionic molecules) the transition frequency is very sensitive the ρ.
The complete description of optical spectra of a DA chromophore requires the introduction of molecular vibrations. We account for a single effective co- ordinate q that linearly modulates the diagonal energy z0(Holstein coupling).
The total Hamiltonian then reads :
H = Hel+ Hph+ He−ph
= 2z0ρ − τ ˆˆ σ +ωv2
− gp2ωvq ˆρ (1.11) where the p is the momentum associated to the q coordinate. ωv is the vi- brational frequency and g is the electron-phonon (e-ph) coupling constant:
q eq. The strength of the coupling is conveniently measured by ǫv=ωg2
v, i.e. the vibrational relaxation energy.
In the adiabatic approximation the vibrational kinetic energy is neglected and q becomes a classical coordinate. In this approximation the total Hamilto- nian: Hadiab=2
ρ − τ ˆˆ σ +12ωv2q2can be easily solved as a two state electronic Hamiltonian with a q dependent z0. The adiabatic solution leads to q dependent |g〉 and |e〉 states and to q dependent energies, that describe the potential energy surfaces (PES), as shown in the right panel of figure 1.3.
The vibrational problem can be solved on each PES to find relevant vibrational eigenstates. As it can be seen in fig. 1.3, the two basis state have harmonic PES with the same curvature, but the PES resulting from the diagonalization are anharmonic and show different curvature. The solution of the vibrational problem becomes trivial if the harmonic approximation is enforced, i.e. if the anharmonic PES for the g and the e state are approximated by parabolic sur- faces. The exact solution of the adiabatic anharmonic problem is possible, but numerically cumbersome.
To deal with the problem in a non adiabatic picture it is useful to introduce raising and lowering operators (ħh = 1) in order to express ˆq and ˆp:
ˆq = 1 p2ωv
ˆp = i 1 p2ωv
Equation 1.11 can be rewritten:
H = Hel+ Hph+ He−ph
= 2z0ρ − τ ˆˆ σ + ωv
− g aˆ†+ ˆa
The total Hamiltonian matrix is then written on the basis obtained as the direct product of the two electronic basis states (|DA〉 and |D+A−〉) times the eigen- states of the harmonic oscillator described by Hph=ωv
aˆaˆ †+12. The result- ing basis set is infinite and is truncated accounting for just the lowest N states
10 Essential state models
-10 0 10
-10 0 10
ωge D A
Figure 1.3: Left: the q-dependent energies of the two electronic basis states. Right:
adiabatic eigenstate PESs obtained from the diagonalization of Hamiltonian in equation (1.11). The figure is obtained for z = 1 eV , τ = 0.5 eV , ωv=0.2 eV and ǫv=0.4 eV. In the left panel, ǫvmarks the vibrational relaxation energy relevant to the basis states, while λv in the right panel, shows the same quantity (i.e. the vibrational relaxation energy) for the adiabatic eigenstates.
of the harmonic oscillator. Numerically exact solutions are obtained by diago- nalising the Hamiltonian matrix on a basis with large enough N as to ensure convergence of the relevant results.
So far we have described an isolated chromophore: to complete the picture we have to account for the interaction between the molecule and its environ- ment. The simplest approach starts studying the molecule in solution. Ignoring all specific effects, we adopt the a reaction field model. A solvent around a polar solute generates an electric field FR that is proportional to the dipole moment of the solute: FR=r〈µ〉. There are two contributions to the reaction field:
FR=FR,el+FR,or=rel〈µ〉 + ror〈µ〉 (1.15) The first contribution accounts for the polarisation of the electronic cloud of solvent molecules around the polar solute. It is related to very fast degrees of freedom (the energy of typical electronic excitations of the solvent, in the UV region) and can be treated in the anti-adiabatic approximation, leading to a renormalisation of the electronic model parameters, τ and z0. FR,el is related only to the refractive index of the solvent, and in view of the minor variability of the refractive index of common organic solvents, we assume that the renor- malized τ and z0parameters are essentially solvent independent.
The second contribution, FR,or, is present only in polar solvent and is due to the reorientation of the polar solvent molecules around the polar solute. This term is characterised by a much slower dynamics compared to the relevant de- grees of freedom and can be accounted for in the adiabatic approximation. We define the solvent relaxation energy ǫor = 12rorµ20 and introduce an effective solvation coordinate f = forµ0, so that the complete Hamiltonian reads:
H = Hel+ Hph+ He−ph− f ˆρ + 1
The parameter ǫor is directly related to the solvent polarity. Polar solvents have large relaxation energies and large value of ǫor, while apolar solvents have ǫor=0. ǫor is the only parameters that determines the evolution of the spectral properties of the chromophore increasing the solvent polarity, and fully accounts for solvatochromism.
In eq. 1.16 the Hamiltonian is parametrically dependent on the solvation coordinate f . The relevant energies describe the potential energy surface (PES) with respect to the f coordinate, with minima centred at the equilibrium value for f , feq=2ǫor〈ρ〉. We treat f as a classical coordinate, so that states around the minimum along each PES are populated with probability pc(f )according to the Boltzmann law:
R pc f′
d f′ (1.17)
where c refer to the electronic considered state (c = g, e).
Therefore to calculate the properties (including optical spectra) of chro- mophore in solution, we diagonalise the f dependent H in eq. 1.16 for different f values and calculate the f dependent property of interest. Ensemble proper- ties are finally obtained summing up on a grid of f values and weighting rel- evant contributions according to the Boltzmann distribution. Along these lines it become obvious that polar solvation is responsible for inhomogeneous broad- ening of optical spectra. Since ǫordetermines the curvature of the f dependent PES, as in eq. 1.16, polar solvents results in larger broadening, while apolar solvents (ǫor≈ 0) corresponds to steep surface with a very deep minimum. Of course the distribution is different for absorption and fluorescence spectra: for absorption spectra the solvent feels the field generated by the the ground state dipole and the distribution has to be calculated based on the ground-state PES;
for fluorescence, the solvent relaxes after excitation, and the distribution has to be calculated based on the excited-state PES.
We underline that in the calculation of optical spectra one must assign a spe- cific lineshape to each transition, calculated at each F value. In particular we
12 Essential state models
f solvatation coordinate [τ unit]
0 1 2 3 4
energy [τ unit]
εor εor = 0.05 εor = 0.25 εor = 0.75 basis state D A and D+ A-
f solvatation coordinate [τ unit]
eigenstate g and e
Figure 1.4: Energy as a function of the orientational solvation coordinate, calcu- lated for model parameter z0=1 (and ǫv=0), with all energies in unit of τ. On the left panel the basis states (called diabatic); on the right the eigenstates (adia- batic states). The dashed lines refer to the excited state energy. It can be noticed the effect of the increase of the solvation relaxation energy ǫor in determining the curvature and the position of the minima (the more polar is the state, the more shifted is the equilibrium position
assign either a Gaussian line to each vibronic band, calculated for each f with a fixed width Γ, independent on the solvent polarity. An estimate of Γ can be obtained from the width of the vibronic lines in non polar solvents. In polar sol- vents, summing over spectra calculated at different f leads to inhomogeneous broadening of the bands.
The detailed procedure to calculate linear and non-linear spectra is explained in appendix sect. B.1.1.
1.2 Essential state models for chromophore and multichromophore
Essential state models account for a minimal set of electronic states and thanks to this simplification, they offer a way to treat in good detail the coupling of electronic and vibrational degrees of freedom and the effects of polar solvation.
Essential state models are semi-empirical models: model parameters must be extracted from the experiment. Most often the parameters are extracted from the analysis of linear optical spectra and from their solvent dependence. Linear and non linear spectra can be calculated with the guessed parameters and the results compared with the experimental one, in a procedure similar to a fit.
Because solvent effects are explicitly accounted for, in essential state ap- proaches the model for the solute molecule is strictly solvent independent. The essential molecular model resulting from the analysis of solution spectra can then be used to describe the same chromophore in different environments. This is the basis for the so called bottom-up approach modelling strategy to describe multichromophoric assemblies [20, 23, 25], molecular films , or crystals [24, 41].
Adopting solvent-independent molecular parameters largely reduces the num- ber of free parameters with respect to standard treatments based on the Marcus- Hush or Jortner models [42, 43, 44, 45, 46]. As it will be underlined in several cases in this chapter, despite of the reduction of free parameters, the calculated spectra satisfactorily reproduce experimental data, confirming the validity of the model. Moreover, the global fit of optical spectra in solvents of different polarity allows for a reliable partitioning of the relaxation energy into a vibrational and a solvation contribution, a delicate issue in the Marcus-Hush treatment where spectra measured in different solvents are analysed separately.
14 Essential state models
DA chromophores beyond the two state approach
The two state model described in sect. 1.1 is a simple and effective model, that has been successfully applied to describe several families of push–pull chro- mophores. It reproduces linear and non-linear properties of DA chromophore in solution and in more complex environments. However, the two-state approxi- mation is quite dramatic and in some experimental systems it must be relaxed.
In this chapter we discuss two examples:
• an organic ligand that is well described as a DA chromophore, but that upon complexation on Zn2+ show an interesting enhancement of the TPA intensity that cannot be explained in a two state model (see sect. 1.3)
• an organic chrysenic-like DA compound whose spectra show a competition between a CT and a localised transition (see sect. 1.4)
Indeed another example of an improved description of a DA molecule be- yond the two state model will described the next chapter, when the role of bridge state is discussed with reference to two chromophores of interest for bistability (see sect. 2.1.7).
1.3 Terpyridine-based ligand and the related Zn- complex
Fig. 1.5 shows the chemical structure of an organic terpyridine–based ligand T and of its Zinc complex [ZnT]. The ligand itself is a push-pull chromophore where the terpyridine group acts as an electron-acceptor, while the amino group is the electron-donor. In the complex the Zinc is coordinated to the acceptor group, leading to a much stronger acceptor character of the complexated ter- pyridine group. Here we combine an essential state model description and a bottom up modelization approach. This work has been done in collaboration with the group of D. Roberto of the University of Milano (Italy) that devel- oped the synthesis of the two compounds, while the nonlinear characterisation (two-photon absorption) was performed by the group of Prof. C. Ferrante of the University of Padova (Italy). Our group is responsible for collecting optical linear spectra, and for the theoretical model .
Figure 1.5: Studied terpyridinic ligand and the related Zinc complex
1.3.1 Ligand: spectroscopy and two state model
Fig. 1.6 (upper panels) reports experimental spectra of the ligand T. Panel (a) shows linear absorption and fluorescence spectra collected in solvents of dif- ferent polarity; panel (b) shows TPA spectra collected in CH2Cl2. Table 1.1 summarizes main spectroscopic data. Linear spectra were collected in our lab- oratory, according to the procedures described in the appendix sect. A.1. The experimental procedures adopted for fluorescence quantum yield (FQY) and TPA measurements done in Padova are explained in appendix A.2.
16 Terpyridine-based ligand and the related Zn-complex
Table 1.1: Experimental data for T in cyclohexane, toluene and dichloromethane.
solvents λabs/nm λf luo/nm λTPA/nm (ε/M−1cm−1) (FQY) (σTPA/GM)
cyclohexane 348 377
toluene 358 413
dichloromethane 362 474 730
(21300±500) (0.27±0.03) (96±12)
One-photon absorption (OPA) and fluorescence spectra were collected in cyclohexane (CH) , toluene and dichloromethane. Since T exhibits very low solubility in CH, for this solvent the spectrum reported in fig. 1.6(a) is not the absorption spectra but the fluorescence excitation spectrum (see caption of fig. 1.6). As expected for a largely neutral polar chromophores, T shows a weakly solvatochromic absorption while fluorescence spectra exhibit a stronger solvatochromism. The TPA band exactly overlaps the linear absorption band (fig. 1.6(b)), as expected for asymmetric molecules.
The two-state model presented in the previous section applies very well to T, as demonstrated by calculated spectra shown in panels (c) and (d) of Figure 1.6, The spectra have been obtained with model parameters in table 1.2 (for de- tails about the calculation of linear and two-photon spectra see appendix B.2).
The results are very good: not only transition energies, but also the evolution of absorbance and fluorescence band shape with solvent polarity are well re- produced. The TPA spectrum is also reproduced quantitatively with the same parameters: in particular we notice that both the molar extinction coefficient of OPA and the TPA cross section are in good agreement with the experimental data. We underline that six parameters of the model (η,p
2t, µ0, ǫv, ωvand the intrinsic linewidth of the vibronic transition, Γ) are solvent-independent, while only one (ǫor) changes with solvent polarity.
1.3.2 Optical spectra of [ZnT]: the need for an extension of the model
The complexation of T on ZnCl2 has interesting consequences in optical spec- tra, as seen in Figure 1.7 (Table 1.3 summarizes experimental data). Absorption and fluorescence spectra are red-shifted with respect to the ligand and the mo- lar extinction coefficient increases by a factor ∼1.2, while the cross section of
20000 25000 30000 wavenumber (cm-1)
ε (M-1 cm-1 )
εor=0.10eV εor=0.39eV εor=0.65eV
0 100 200
20000 25000 30000
20000 25000 30000 wavenumber (cm-1)
0 100 200
σTPA (GM) 0
ε (M-1 cm-1 )
Cyclohexane Toluene CH2Cl2
Figure 1.6: Top panels: experimental spectra of T. Panel a: continuous and dashed lines refer to absorption and fluorescence, respectively. T hardly dissolves in CH, and in the OPA spectrum a very weak band appears in the low-energy region that can be assigned to the complexation of T with traces of metallic ions in solution. To overcome this problem, the fluorescence excitation spectrum is shown (black con- tinuous line, in arbitrary units). The molar extinction coefficient was measured in CH2Cl2and spectra collected in other solvents are normalised to this value. Panel c:
TPA spectrum in Göppert-Mayer (symbols and errors bars) and OPA spectrum (ar- bitrary units, dotted line) collected in CH2Cl2. Bottom panels: Spectra calculated for T by the two-state model using the parameters reported in Table 1.2
18 Terpyridine-based ligand and the related Zn-complex
Table 1.2: Model parameters for [ZnT] and for T: the molecular parameters rel- evant to the T ligand (τ, z0, µ0, ωv, εv and Γ) are rigidly transferred from the two-state model to the three state model (common values, upper part of the ta- ble). In the central part of the table are shown the parameters entering only the three-state model for [ZnT] and in the last part the solvent parameters for both molecules .
molecular parameter T [ZnT]
solvent parameter T [ZnT]
ǫor/eV cyclohexane 0.10
toluene 0.39 0.13
dichloromethane 0.62 0.27
20000 25000 30000 wavenumber cm-1
ε (M-1 cm-1 )
0 100 200
20000 25000 30000 wavenumber cm-1
0 100 200
σTPA (GM) 0
ε (M-1 cm-1 )
emission (a.u) εor=0.13 eV
Figure 1.7: Top panels: experimental spectra of [ZnT]. Panel a: continuous and dashed lines refer to absorption and fluorescence, respectively. The molar extinc- tion coefficient was measured in CH2Cl2and spectra collected in other solvents are normalises to this value. Panel c: TPA spectrum in GM (symbols and error bars) and OPA spectrum (arbitrary units, dotted line) collected in CH2Cl2. Bottom pan- els: Spectra calculated for [ZnT] by the three-state model using the parameters reported in Table 1.2
20 Terpyridine-based ligand and the related Zn-complex
Table 1.3: Experimental data for [ZnT] toluene and dichloromethane.
solvent λabs/nm λf luo/nm λT PA/nm (ε/M−1cm−1) (FQY %) (σTPA/GM)
toluene 405 463
dichloromethane 427 549 847
(25700±400) (0.48±0.05) (186±24)
two-photon absorption increases by a factor of ∼2 with respect to T . Linear optical properties of [ZnT] can be rationalised in the two state picture: upon complexation with the Lewis acid group ZnCl2, the acceptor strength of the ter- pyridine group increases lowering the energy of D+A−, and therefore decreasing the z0value. As a results ρ increases justifying the red shift of the absorbance and fluorescence bands as well as the the weak increase of the absorption inten- sity. But when we tried to reproduce the increase seen in the TPA cross section, the two state model fails completely: in fact we obtain an amplification of the TPA cross section not larger than 1.2. The reason for the failure of the two-state model for [ZnT] has to be ascribed to the presence of a higher-energy state, that contributes to the TPA response, while barely affecting the low-energy state in- volved in OPA.
Then we model [ZnT], again in an essential-state picture, as a DAAvspecie, where Av is a virtual acceptor that mimics the ZnCl2group. This leads to three resonating structures:
D A Av←→ D+A−Av←→ D+A A−v
that define three basis states. In agreement with the two-state model, the states
|D A Av〉 and |D+A−Av〉 are separated in energy by 2z0and the mixing element is −τ. The energy gap between D+A−Av and D+A A−v is 2(x0− z0), and the two states are mixed by −τ′, as sketched in Figure 1.8. The corresponding Hamiltonian is:
0 −τ 0
−τ 2z0 −τ′ 0 −τ′ 2x0
|D+A A−v〉 is a virtual high-energy state (x0 > z0), that, being not directly coupled with the neutral state |D A Av〉, marginally affects the ground state.
On the other hand, |D+AA−v〉 significantly contributes to the first excited state, leading to a sizeable increase of the dipole moment of the first excited state,
Figure 1.8: The three basis states for [ZnT]
and hence of ∆µ = µe− µg. The OPA intensity is proportional to the squared transition dipole moment (µ2ge) between the ground state and the excited state, and is barely affected by the presence of the virtual state. On the other hand, the TPA cross section is proportional to ∆µ2µ2ge, so that a sizeable increase of the TPA response is expected as a result of complexation, as experimentally observed .
Before starting the detailed analysis of optical spectra of the [ZnT] complex, the role of the virtual state on the intensity of OPA and TPA spectra is discussed in more detail. Colour maps in Figure 1.9 show the OPA (top panel) and the TPA intensities (bottom panel) calculated as a function of z0 (half the energy gap between D A Avand D+A−Av) and of x0− z0(half the energy gap between D+A−Avand D+A A−v, figure 1.8), for the three state model in Eq. 1.19. Both the mixing elements are set to 1 (τ = τ′=1) and the dipole moment of D+A A−v is set to 2µ0, twice the dipole moment of D+A−Av. For x0−z0≫ τ′the virtual state becomes irrelevant, and one regains the two-state model. In particular for small values of z0, ρ → 0.5 and according to equation 1.7 (and fig. 1.9) the transition dipole moment is very large, so that the OPA intensity is high. Increasing z0, the system becomes more neutral, ρ decreases, and OPA decreases as well. Anyway, the presence of the virtual excited state never affects the OPA intensity signifi- cantly. On the contrary, the TPA intensity strongly depends on the energy of the virtual state, and, as shown in the bottom panel of Figure 1.9, it increases when the virtual excited states approaches the first excited state. These predictions suggest that the three-state model can explain the experimental observations.
For a more detailed modelling of the [ZnT] complex, molecular vibrations and polar solvation are introduced, along similar lines as previously discussed for the two-state model. Again, only one effective molecular coordinate is cou- pled to the electronic transition, with frequency ωv and relaxation energy ǫv.
22 Terpyridine-based ligand and the related Zn-complex
0.5 1 1.5 2
0.5 1 1.5 2
0.3 0.4 0.5 0.6 0.7 0.8 0.9
0.5 1 1.5 2
0.5 1 1.5 2
50 100 150 200 250 300 350 400
Figure 1.9: Results of the three-state electronic model with τ = τ′ =1 eV, µ0= 20D and α = 2. Colour maps show the OPA intensity as calculated oscillator strength (top panel) and TPA intensity in GM estimated at the maximum of the TPA band (bottom panel) as function of z0and x0− z0for the first electronic state, using the three-state model The red contour lines mark the equispaced levels, with increments 0.1 and 50GM in the top and bottom panel, respectively. This refers to pure electronic problem (ǫor =0and ǫv=0). Effective width was introduced to estimate numerically the cross section: Γe f f=0.16 eV .
We assume for the |D+A A−v〉 state the same coupling as for the |D+A−Av〉 state.
The electronic and vibrational Hamiltonian then reads:
Hel+ He−ph+ Hph =
0 −τ 0
−τ 2z0− ωvp2ǫvq −τ′ 0 −τ′ 2x0− ωvp2ǫvq
(1.19) The reaction field approach is followed to account for polar solvation. Be- cause of the coordination with the polar ZnCl2 we account for its permanent dipole moment introducing a parameter µ′. Moreover to measure the dipole length of |D+AA−v〉 we introduce a parameter α (α > 1 on physical basis) so that the dipole moment operator reads:
ˆ µ =
µ′ 0 0
0 µ′+µ0 0 0 0 µ′+αµ0
We notice that µ′ does not affect OPA and TPA intensities (it does not enter the transition dipole moments nor the mesomeric dipole moment), but it is responsible for a larger solvatochromism of absorption bands with respect to T.
With this hypothesis for the dipole moments, the three-state Hamiltonian reads:
H = Hel+ He−ph+ Hph+ 1
µ0µ f +ˆ 1
4ǫorf2 (1.21) As for two state model we treat f as a classical variable. For fixed f the H in Equation 1.21 defines a coupled electron-vibration problem that is numerically diagonalised on a non-adiabatic basis. The spectra are calculated as described in appendix B.
The number of parameters entering the three-state model is large and to re- duce the number of freely adjustable parameters we exploit the bottom-up mod- elling strategy and transfer all relevant parameters from the two-state model of a free ligand T to the description of the ligand unit within the complex. Table 1.2 summarizes all parameters entering T and [ZnT] model. Molecular param- eters τ, z0, µ0, ωv, ǫv and Γ in the first part of the table, are common to the two molecules. Solvent relaxation energies are smaller than those reported for T, a fact that can be rationalised in terms of the smaller dimension of the so- lute cavity for T than for [ZnT]. Calculated spectra are reported in the bottom panels of fig. 1.7. The agreement with experimental data is very good: band shapes, transition energies and intensities (molar extinction coefficients and the TPA cross section) are well reproduced.
24 Terpyridine-based ligand and the related Zn-complex
Quite interestingly the three-state model actually accounts for the inductive effects predicting a red-shift of the optical transition without the need to empir- ically re-adjust z0. The third state D+AA−v included in the model, can be defined as a virtual state in the sense that it marginally affects the ground state and lin- ear spectral properties. However it does enter with sizeable weight the first ex- cited state, leading to an increase of the dipole moment of the first excited state, and hence to an amplification of the TPA response, where σTPA∝ µ2ge(µg− µe)2 (see appendix B). This mechanism is general, and can be extended to different systems: attaching a virtual acceptor or a virtual donor to a push-pull chro- mophore is expected to sizeable increase its TPA response.
1.4 Annine: CT vs localized excitations
In collaboration with S. Quici (CNR-Milano), D. Roberto (University Milano) and C. Ferrante (Padova) we have investigated a family of chrysene derivative molecules. The molecular structure of these molecules in fig. 1.10 is charac- terized by an extendend π framework, that in virtue of its rigidity lead to good photostability. The properties of molecules in this family have been already object of some investigation [48, 49].
Figure 1.10: Chemical structures of the molecules discussed in this section
An is an heterocyclic substituited chrysene in which the carbon in position 2 is substituited with a nitrogen atom, obtaining the corresponding 2-azachrisene and increasing the acceptor strength of the substituted ring. An represent the reference compound. Adding an electron donor group on the opposite side of the fused ring structure, we obtain the 8-N,N-dibutylamino-2-azachrysene (NAn), as in figure 1.10, that represent an interesting DA chromophore. The third compound, NAnM+, from which the family name ANNINE comes (ANel- lated benzene rings hemicyaNINE), is obtained by methylation of the pyridinic nitrogen, resulting in a strong increase of the acceptor strength. We describe in detail the properties of NAn, the parallel study of An and NAnMe+ is mainly realized to support our analysis of NAn.
1.4.1 Optical properties of An
We study the compound An (2-azachrisene, show in figure 1.10) in order to support the physical interpretation of the NAn spectra, that will be described later. Absorption and fluorescence emission and fluorescence excitation spectra of An are measured in cyclohexane, toluene, CH2Cl2and DMSO.
We encounter some difficults related to the poor solubility of An in almost all solvents, an to its the tendency to form aggregates and/or excimers .
Fluorescence excitation spectra are helpful in this respect. Anyway, in diluite solutions and/or after sonication and filtration a set of reliable spectra was ob- tained, except for cyclohexane. Results are shown in figure 1.11. The presence
26 Annine: CT vs localized excitations
of a bad baseline for toluene, as well as the unresolved low energy side of the emission spectra can be due to formation of aggregates and excimers.
20000 25000 30000
absorbance (a. u.)
toluene CH2Cl2 (exc.) DMSO
emission intensity (a.u.)
Figure 1.11: Experimental absorption and fluorescence of An in three solvent. For CH2Cl2the excitation spectra is shown instead of the absorption.
Anyway, spectra in fig. 1.11 show the typical behaviour expected for organic conjugated fused ring chromophores, with π → π∗excitations with narrow and well resolved vibronic structure. The negligible effect of the solvent polarity on optical spectra, showing no broadening and no solvatochromism upon in- creasing solvent polarity, confirms the localized nature of the excitations and the emission.
1.4.2 Optical properties of NAn
Linear optical spectra (absorbtion and fluorescence) of NAn were collected in solvents of different polarities: cyclohexane, toluene, CH2Cl2and DMSO. Molar extinction coefficient and FQY were also measured in CH2Cl2and DMSO. Spec- tra are shown in fig. 1.12 e 1.13 and spectroscopic quantities are summarized in tables 1.4 and 1.5. The absorption spectrum is characterized by three systems of transitions (see fig. 1.12):
• a weak absorption I at∼ 410 nm, that is well resolved in nonpolar solvent
• a band at about 350-360 nm (II), with a distinct solvatochromic behaviour
• a strong peak at∼ 300 nm (III)